Nonferrous_4Ed-Arc Welding of Nonferrous Metals
out of 83
Post on 29-Dec-2015
<ul><li><p> Arc Welding ofNonferrousMetals</p><p>FOURTH EDITION</p><p>Published by</p></li><li><p> Arc Welding ofNonferrousMetals</p><p>FOURTH EDITION</p><p>Kita-Shinagawa, Shinagawa-Ku, Tokyo, 141-8688 Japan</p></li><li><p>Published by KOBE STEEL, LTD. </p><p> 2011 by KOBE STEEL, LTD. </p><p>5-912, Kita-Shinagawa, Shinagawa-Ku, Tokyo, 141-8688 Japan </p><p> All rights reserved. </p><p>No part of this book may be reproduced, in any form or by any means, without </p><p>permission in writing from the publisher </p><p> The Arc Welding of Nonferrous Metals is a textbook for providing information to assist welding personnel study the arc welding technologies commonly applied in the equipment made from aluminum, aluminum alloys, copper, copper alloys, nickel, and nickel alloys. Reasonable care is taken in the compilation and publication of this textbook to insure authenticity of the contents. No representation or warranty is made as to the accuracy or reliability of this information. </p></li><li><p> iii</p><p> Forewords Nonferrous metals are non-iron-based metals such as aluminum and aluminum alloys, copper and copper alloys, nickel and nickel alloys, titanium and titanium alloys, and magnesium and magnesium alloys. Today, nonferrous metals are used in various welding constructions for diverse industrial applications. However, their weldability is quite different from that of steel, due to specific physical and metallurgical characteristics. Therefore, the welding procedure for nonferrous metals should be thoroughly examined taking into account the inherent characteristics of the particular nonferrous metal to be welded, in order to get sound weldments. This textbook focuses on the arc welding of aluminum, aluminum alloys, copper, copper alloys, nickel, and nickel alloys that are used more extensively over other nonferrous metals for industrial applications. This textbook consists of three chapters: </p><p>Chapter 1: Arc Welding of Aluminum and Aluminum Alloys Chapter 2: Arc Welding of Copper and Copper Alloys Chapter 3: Arc Welding of Nickel and Nickel Alloys </p></li><li><p>Contents Introduction 2 1.1 General characteristics 3 1.2. Wrought products 5 1.2.1 Nonheat-treatable type 6 1.2.2 Heat-treatable type 6 1.2.3 Chemical and mechanical properties 7 1.3 Casting products 10 2.1 Weldability of aluminum and aluminum alloys 11 2.2 Filler metal selection 14 3.1 Gas tungsten arc welding 16 3.2 Gas metal arc welding 19 3.3 Welding groove preparation 21 3.4 Welding conditions 24 3.5 Welding distortion and countermeasures 26 3.6 Weld discontinuities and preventive measures 29 </p><p>1. Types and features of aluminum and aluminum alloys 3 </p><p>2. Weldability and filler metal selection 11 </p><p>3. Welding processes and procedures 16 </p><p> Arc Welding </p><p>of Aluminum and Aluminum Alloys </p></li><li><p> Arc Welding of Aluminum and Aluminum Alloys </p><p>2 </p><p> Introduction Nowadays, aluminum and aluminum alloys are extensively used for various applications such as household utensils, autos, railroad cars, buildings, bridges, aircrafts, spacecrafts, ships, chemical equipment, water gates, and storage tanks, because of the inherent advantages of high strength-to-weight ratio, high notch toughness at cryogenic temperatures, excellent corrosion resistance, ease in extrusion, and good fabricability. Aluminum and its alloys are readily joined with most of the known joining processes including welding, brazing, soldering, adhesive bonding, and mechanical fastening. Of these joining processes, welding is most widely used. The welding processes used for aluminum and its alloy assemblies are arc welding, stud welding, electron beam welding, laser beam welding, resistance welding, solid-state welding, and oxyfuel gas welding. Of these welding processes, arc welding is most extensively used. The arc welding processes used commonly in the assemblies are gas tungsten arc welding (GTAW) and gas metal arc welding (GMAW). Basically, aluminum and its alloys can successfully be arc welded by using conventional GTAW/GMAW equipment and techniques used for other metals, provided the welding procedure is suitable. However, occasionally specialized equipment or techniques, or both, are required due to the inherent unique physical and mechanical characteristics of aluminum and its alloys. This section focuses on GTAW and GMAW of aluminum and its alloys and discusses diverse types of such metals and their weldability, suitable welding equipment, proper filler metals and welding procedures, and provides tips for sound welds. </p><p> References  The Japan Light Metal-Welding and Construction Association, Introductory Course for Inert Gas Arc Welding of Aluminum (Alloys), 2001  The American Welding Society, Welding Handbook, 8th Edition, Vol. 3, 1996  A. Kamio, The New Era of Aluminum, 1999, Kogyo Chosakai Publishing Co., Ltd.  Kobe Steel, Ltd., Welding Electrodes Handbook, 1964  The Japan Welding Engineering Society, Seminar Textbook for ISO 14731/WES 8103 </p><p>Welding Coordination Personnel Certification Renewal, 2002  M. Mizuno, et. al., Welding of Aluminum and Aluminum Alloys, Sanpo Publications Inc., 1979  Shinko Welding Service Co., Ltd., Exposition of Welding Terms, 1999  T. Tachibana, Materials and Procedures for Aluminum MIG Welding, Journal of the Japan </p><p>Welding Society, Vol. 70, No. 3, 2001  The American Welding Society, Welding Handbook, 8th Edition, Vol. 2, 1991  Kobe Steel, Ltd., Technical Guide, No. 344, 1998 </p></li><li><p>Arc Welding of Aluminum and Aluminum Alloys </p><p> 3</p><p>1. Types and features of aluminum and aluminum alloys Aluminum and aluminum alloys are the lightest commercial metals in use in large quantities. Aluminum is easy to extrude and fabricate and has excellent corrosion resistibility. Various types of aluminum alloys are also available in response to demands for higher strength and superior corrosion resistibility for specific applications. This chapter discusses general characteristics, types and features of aluminum and its alloys. 1.1 General characteristics The applications of aluminum and its alloys are expanding in various industrial fields because of its many advantages over other metals. The following paragraphs discuss the advantages of aluminum and its alloys for structural material. Table 1.1 shows a comparison of physical properties between aluminum and mild steel. (1) Lightweight: </p><p>As shown in Table 1.1, the density of aluminum is 2.7, which is about 1/3 of that of mild steel (7.86). This feature is one of the reasons why aluminum and its alloys are widely used for transportation vehicles such as autos, railway cars (Photo 1.1), aircrafts, and ships (Photo 1.2). By decreasing the weight of the transportation vehicles the energy consumption efficiency can be improved. </p><p>Photo 1.1Shinkansen high-speed trains uses plates, extrusions, castings and forgings of aluminum alloy (Source: Kobe Steels brochure) </p><p>Photo 1.2A fishing boat made of aluminum alloy </p><p>structural components.(Source: Kobe Steels brochure)</p></li><li><p> Arc Welding of Aluminum and Aluminum Alloys </p><p> 4</p><p>(2) Strong: The tensile strength of aluminum is much lower than that of mild steel; </p><p>however, it can readily be strengthened by alloying with other elements such as copper, manganese, silicon, magnesium, and zinc. Aluminum and its alloys can further be strengthened by cold working (rolling, extrusion, drawing and forging), due to work hardening or strain hardening. The certain group of aluminum alloys can be strengthened by precipitation hardening heat treatment. With this treatment, the tensile strength of some alloys becomes comparable to or even higher than that of mild steel. </p><p> With lower specific gravity, the ratio of strength to specific gravity of many </p><p>aluminum alloys is higher than that of mild steel. This advantage is useful particularly for transportation vehicles such as aircrafts, spacecrafts, autos, railroad cars, and boats. </p><p> (3) High resistance to corrosion: </p><p>Aluminum forms an oxide film (alumina) on its surfaces in the air. This oxide film is thin but dense enough to protect the base metal in corrosive atmospheres and solutions. In addition, alloying with magnesium provide aluminum with much higher resistance to corrosion. This is why aluminum alloys are extensively used in buildings, ships, and autos. </p><p> (4) Good workability: </p><p>Aluminum and its alloys can readily be formed plastically by rolling, extrusion, and forging. Aluminum alloys containing silicon have excellent castability. This is why products range with a wide variety including plates, extrusions (Photo 1.3), rods, wires, forgings and castings (Photo 1.4). </p><p>Photo 1.3 An extrusion of aluminum alloy for railroad car components (Source: Kobe Steels brochure) </p><p>Photo 1.4Forgings and castings of aluminum alloy </p><p>for automobile components(Source: Kobe Steels brochure)</p></li><li><p>Arc Welding of Aluminum and Aluminum Alloys </p><p> 5</p><p>Table 1.1. A comparison of physical properties between aluminum and mild steel [Ref. 6] </p><p>Physical properties Aluminum (99.9% or higher Al) </p><p>Mild steel (JIS SS400) </p><p>Density (g/cm3) 2.7 7.86 Melting point () 660 1500-1527 Average specific heat (0-100)(cal/g/) 0.22 0.11 Expansion coefficient (20-100) (106 ) 24 12 Thermal conductivity (cal/cm/s/) 0.52-0.54 0.12 Elasticity modulus (kgf/mm2) 6000-7000 21000 Shear modulus (kgf/mm2) 2500 8400 Latent heat of fusion (cal/g) 97 66 </p><p> (5) Good heat conductivity: </p><p>The thermal conductivity of aluminum and its alloys are about 3-4 times as large as that of mild steel. Therefore, aluminum can be hot by heating or cold by cooling more quickly than steel. This is why aluminum and its alloys are used for air conditioning equipment, combustion engine components, heat exchangers, and radiators. </p><p> (6) Excellent notch toughness at cryogenic temperatures: </p><p>Aluminum alloys are often used for cryogenic temperature process plants and LNG storage tanks because aluminum alloys offer high notch toughness at cryogenic temperatures (196 for liquefied nitrogen, 183 for liquefied oxygen, and 162 for liquefied natural gas), thereby preventing brittle fracture of the equipment. </p><p> (7) Readily weldable: </p><p>With exception of some aluminum alloys, aluminum and its alloys are readily arc weldable. This is why a variety of constructions can be effectively fabricated. </p><p> 1.2 Wrought products Wrought aluminum and aluminum alloy products include plate, bars, shapes, pipes, wires, forgings, and foils. They are produced by plastic working processes such as rolling, extrusion, drawing, and forging, subsequent to the melting and casting processes. As shown in Table 1.2, the means by which the alloying elements strengthen aluminum is used to classify aluminum and its alloys into two groups: the nonheat-treatable and heat-treatable. They are also classified by the purity and main alloying elements with a four-digit numerical designation system. The first digit indicates the aluminum and aluminum alloy series. The second digit in individual series indicates consecutive modifications of an original type (0) of aluminum and its alloys; N is for the Japanese origin. For 1XXX series, the last two digits indicate the minimum aluminum purity (e.g., 1100: 99.00%Al min.). </p></li><li><p> Arc Welding of Aluminum and Aluminum Alloys </p><p> 6</p><p>Table 1.2 Classification of wrought aluminum and aluminum alloy products Alloy group Alloying </p><p>system Designation system Alloy </p><p>designation (1) </p><p>Nonheat-treatable type </p><p>Al: 99.00% min Al-Mn Al-Si Al-Mg </p><p>1XXX 3XXX 4XXX 5XXX </p><p>1100 3003 4043 5005, 5052, 5083 </p><p>Heat-treatable type Al-Cu Al-Mg-Si Al-Zn-Mg </p><p>2XXX 6XXX 7XXX </p><p>2219 6061, 6N01, 6063 7003, 7N01 </p><p> Note (1) The alloy designations are as per the JIS H 4000-999 (for plates and strips), JIS H 4100-1999 (for shapes) and JIS Z 3232-2000 (for welding rods and wires). 1.2.1 Nonheat-treatable type Nonheat-treatable aluminum and its alloys cannot be strengthened by heat treatment. The initial strength of the aluminum and its alloys, thus, depends primarily on the effect of silicon, iron, manganese and magnesium contained as impurities or alloying elements. These chemical elements affect increase in strength either as dispersed phases or by solid-solution strengthening. The nonheat-treatable aluminum and aluminum alloy products are mainly found in the 1XXX, 3XXX, 4XXX and 5XXX series. Iron and silicon are the main impurities in commercial aluminum, but they add strength to the 1XXX series. The strength of nonheat-treatable aluminum and its alloys can be increased by strain hardening in cold working processes such as rolling, extrusion, drawing, and forging. In this case, annealing heat treatment (300-400) [Ref. 3] may be applied to relieve strain of the crystals, thereby decreasing the strength and increasing the ductility of the metals. The 5XXX alloys containing magnesium tend to decrease strength and increase ductility by age softening, if they are left for long time after cold working. To prevent the age softening, stabilization heat treatment (130-170 for about 2h) [Ref. 3] is applied. 1.2.2 Heat-treatable type Heat-treatable aluminum alloys are found primarily in the 2XXX, 6XXX, and 7XXX series. The initial strength of the alloys in this group depends on chemical composition, just as in the nonheat-treatable alloys. Alloying elements such as copper, magnesium, zinc, and silicon, either singularly or in various combinations, show a marked increase in solid solubility in the matrix of the alloy with increasing temperature; it is, therefore, possible to subject them to thermal treatments that will impart much strengthening. Mechanical properties of heat-treatable aluminum alloys can be improved by solution heat treatment (450-550 ) [Ref. 3] and subsequent water quenching, followed by natural or artificial aging (100-250) [Ref. 3]. With this series of heat treatments, the alloys increase their strength by precipitation hardening. </p></li><li><p>Arc Welding of Aluminum and Aluminum Alloys </p><p> 7</p><p> The relationship between aging temperature, aging time and Vickers hardness of a heat-treatable aluminum alloy is shown in Fig. 1.1. With a higher aging temperature, a maximum hardness can be attained faster; however, the maximum hardness is lower. In contrast, with a lower aging temperature, the hardness reaches a maximum slower, which is higher than the former. An excessive aging over the time where the maximum hardness is attained decreases hardness thus decreases strength and increases ductility. </p><p> The heat-treatable aluminum alloys may additionally be strengthened by cold working. It may also be annealed to attain maximum ductility. The annealing involves holding the alloy at an elevated temperature and controlled cooling to achieve maximum softening. 1.2.3 Chemical and mechanical properties Table 1.3 shows nominal chemical comp...</p></li></ul>
View more >
The determinants of Chinese nonferrous metals imports and ?· The determinants of Chinese nonferrous…
Arc Welding Metals and Welding. Precautions and Safe Practices Relatively safe compared to other forms of welding 4 areas of concern during arc welding.
ELECTRIC WELDING - WELDING Types – Resistance, Electric arc, gas welding. Ultrasonic, Welding electrodes of various metals, Defects in welding. Introduction
a viewSHIELDED METAL ARC WELDING/FUNDAMENTALS OF THE PROCESS DEFINITION AND GENERAL DESCRIPTION SHIELDED METAL ARC welding (SMAW) is an arc welding process in which coalescence of metals is ...
Interaction of the Refractory Lining of the Hearth of an Electric Arc Furnace with Nonferrous Metals of the Scrap Charge
FUNDAMENTALS OF ARC WELDING - CED of Arc Welding CourFUNDAMENTALS OF ARC WELDING ... Electric arc welding is by far the most popular fusion process for joining metals in ... The resistance of the air or gas between
Shielded Metal Arc Welding and Carbon Arc Cutting Air Metal Arc Welding and Carbon Arc ... identify common metals used for welding Fundamentals of ... Interpret Drawing and Welding Symbols and Written Welding ...